#jsDisabledContent { display:none; } My Account |  Register |  Help

# Mark–Houwink equation

Article Id: WHEBN0014670825
Reproduction Date:

 Title: Mark–Houwink equation Author: World Heritage Encyclopedia Language: English Subject: Collection: Publisher: World Heritage Encyclopedia Publication Date:

### Mark–Houwink equation

The Mark–Houwink equation, also known as the Mark–Houwink–Sakurada equation or the Kuhn–Mark–Houwink–Sakurada equation gives a relation between intrinsic viscosity [\eta] and molecular weight M:[1]

[\eta]=KM^a

From this equation the molecular weight of a polymer can be determined from data on the intrinsic viscosity and vice versa.

The values of the Mark–Houwink parameters, a and K, depend on the particular polymer-solvent system. For solvents, a value of a=0.5 is indicative of a theta solvent. A value of a=0.8 is typical for good solvents. For most flexible polymers, 0.5\leq a\leq 0.8. For semi-flexible polymers, a\ge 0.8. For polymers with an absolute rigid rod, such as Tobacco mosaic virus, a=2.0.

## Applications

In size-exclusion chromatography, such as gel permeation chromatography, the intrinsic viscosity of a polymer is directly related to the elution volume of the polymer. Therefore, by running several monodisperse samples of polymer in a gel permeation chromatograph (GPC), the values of K and a can be determined graphically using a line of best fit. Then the molecular weight and intrinsic viscosity relationship is defined.

Also, the molecular weights of two different polymers in a particular solvent can be related using the Mark–Houwink equation when the polymer-solvent systems have the same intrinsic viscosity:

K_1M_1^{1+a_1}=K_2M_2^{1+a_2}

Knowing the Mark–Houwink parameters and the molecular weight of one of the polymers allows one to find the molecular weight of the other polymer using a GPC. The GPC sorts the polymer chains by volume and as intrinsic viscosity is related to the volume of the polymer chain, the GPC data is the same for the two different polymers. For example, if the GPC calibration curve is known for polystyrene in toluene, polyethylene in toluene can be run in a GPC and the molecular weight of polyethylene can be found according to the polystyrene calibration curve via the above equation.[2]

## References

1. ^ Paul, Hiemenz C., and Lodge P. Timothy. Polymer Chemistry. Second ed. Boca Raton: CRC P, 2007. 336, 338–339.
2. ^ "Gel Permeation Chromatography" California Polytechnic State University. 11 Dec. 2007
This article was sourced from Creative Commons Attribution-ShareAlike License; additional terms may apply. World Heritage Encyclopedia content is assembled from numerous content providers, Open Access Publishing, and in compliance with The Fair Access to Science and Technology Research Act (FASTR), Wikimedia Foundation, Inc., Public Library of Science, The Encyclopedia of Life, Open Book Publishers (OBP), PubMed, U.S. National Library of Medicine, National Center for Biotechnology Information, U.S. National Library of Medicine, National Institutes of Health (NIH), U.S. Department of Health & Human Services, and USA.gov, which sources content from all federal, state, local, tribal, and territorial government publication portals (.gov, .mil, .edu). Funding for USA.gov and content contributors is made possible from the U.S. Congress, E-Government Act of 2002.

Crowd sourced content that is contributed to World Heritage Encyclopedia is peer reviewed and edited by our editorial staff to ensure quality scholarly research articles.